High-pressure high-temperature synthesis and crystal structure of the isotypic rare earth (RE)‒thioborate‒sulfides RE9[BS3]2[BS4]3S3, (RE=Dy‒Lu)
Borna, Marija; Hunger, Jens; Ormeci, Alim; Zahn, Dirk; Burkhardt, Ulrich; Carrillo-Cabrera, Wilder; Cardoso-Gil, Raul; Kniep, Rüdiger; Journal of Solid State Chemistry 184 (2011) 296–303; doi:10.1016/j.jssc.2010.11.004

data_1563308
_publ_section_title
;
 High-pressure high-temperature synthesis and crystal structure of the
 isotypic rare earth (RE)--thioborate--sulfides RE9[BS3]2[BS4]3S3,
 (RE=Dy--Lu)
;
_journal_issue                   2
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              296
_journal_page_last               303
_journal_paper_doi               10.1016/j.jssc.2010.11.004
_journal_volume                  184
_journal_year                    2011
_chemical_formula_moiety         'B3.33 Dy6 S14'
_chemical_formula_structural     'Dy9 (B S3)2 (B S4)3 S3'
_chemical_formula_sum            'B3.33 Dy6 S14'
_chemical_formula_weight         1459.98
_chemical_name_systematic        'Dysprosium thioborate'
_space_group_IT_number           173
_space_group_name_Hall           'P 6c'
_space_group_name_H-M_alt        'P 63'
_symmetry_cell_setting           hexagonal
_symmetry_space_group_name_Hall  'P 6c'
_symmetry_space_group_name_H-M   'P 63'
_cell_angle_alpha                90.0
_cell_angle_beta                 90.0
_cell_angle_gamma                120.0
_cell_formula_units_Z            1
_cell_length_a                   9.4044(2)
_cell_length_b                   9.4044
_cell_length_c                   5.8855(3)
_cell_measurement_reflns_used    54
_cell_measurement_temperature    298
_cell_measurement_theta_max      42.457
_cell_measurement_theta_min      1.500
_cell_volume                     450.79(2)
_computing_structure_refinement  GSAS
_diffrn_ambient_temperature      298
_diffrn_measurement_device_type  'STOE StadiP-MP diffractometer'
_diffrn_radiation_monochromator  'curved germanium (111)'
_diffrn_radiation_polarisn_ratio 0.902
_diffrn_radiation_probe          x-ray
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           'Cu K\a~1~'
_diffrn_radiation_wavelength     1.540598
_exptl_absorpt_coefficient_mu    145.62
_exptl_crystal_density_diffrn    5.381
_exptl_crystal_density_method    'not measured'
_exptl_crystal_F_000             637
_pd_calc_method                  'Rietveld Refinement'
_pd_char_colour                  brown-red
_pd_char_particle_morphology     'size < 0.40mm'
_pd_meas_2theta_range_inc        0.02
_pd_meas_2theta_range_max        109.98
_pd_meas_2theta_range_min        10.0
_pd_meas_number_of_points        5000
_pd_meas_scan_method             step
_pd_phase_name                   'Dy9 B5 S21'
_pd_proc_2theta_range_inc        0.02
_pd_proc_2theta_range_max        109.98
_pd_proc_2theta_range_min        10.0
_pd_proc_ls_background_function
;   GSAS Background function number 1 with 20 terms.
 Shifted Chebyshev function of 1st kind
   1:    1988.08     2:   -704.447     3:    867.371     4:   -223.158    
   5:   -24.2190     6:    76.7823     7:   -30.5126     8:   -12.4041    
   9:    23.0704    10:   -25.0335    11:    10.0644    12:    2.11827    
   13:   -12.7415    14:    13.0308    15:   -5.55881    16:   0.440814    
   17:    6.60261    18:   -8.11003    19:    4.89448    20:   -3.49146        
;
_pd_proc_ls_peak_cutoff          0.00100
_pd_proc_ls_profile_function
;
 CW Profile function number 3 with  19 terms
 Pseudovoigt profile coefficients as parameterized in
 P. Thompson, D.E. Cox & J.B. Hastings (1987). J. Appl. Cryst.,20,79-83.
 Asymmetry correction of L.W. Finger, D.E. Cox & A. P. Jephcoat (1994).
 J. Appl. Cryst.,27,892-900.
 #1(GU)   =    0.000 #2(GV)   =    8.598 #3(GW)   =    9.386
 #4(GP)   =    0.000 #5(LX)   =    4.203 #6(LY)   =    0.000
 #7(S/L)  =   0.0082 #8(H/L)  =   0.0082
 #9(trns) =    -0.46 #10(shft)=   2.8041
 #11(stec)=     4.70 #12(ptec)=    -2.25 #13(sfec)=     0.00
 #14(L11) =    0.051 #15(L22) =    0.027 #16(L33) =    0.220
 #17(L12) =    0.013 #18(L13) =   -0.089 #19(L23) =   -0.072
 Peak tails are ignored  where the intensity is below 0.0010 times the peak
   Aniso. broadening axis   0.0   0.0   1.0
;
_pd_proc_ls_prof_R_factor        0.0261
_pd_proc_ls_prof_wR_expected     0.0239
_pd_proc_ls_prof_wR_factor       0.0370
_pd_proc_number_of_points        5000
_pd_spec_mounting                capillary
_pd_spec_mount_mode              transmission
_refine_ls_goodness_of_fit_all   1.00
_refine_ls_matrix_type           full
_refine_ls_number_constraints    2
_refine_ls_number_parameters     15
_refine_ls_number_restraints     2
_refine_ls_R_Fsqd_factor         0.0989
_refine_ls_shift/su_max          0.06
_refine_ls_shift/su_mean         0.01
_refine_ls_weighting_scheme      calc
_reflns_d_resolution_high        1.000
_reflns_d_resolution_low         8.142
_reflns_limit_h_max              7
_reflns_limit_h_min              0
_reflns_limit_k_max              8
_reflns_limit_k_min              0
_reflns_limit_l_max              5
_reflns_limit_l_min              0
_reflns_number_total             178
_cod_data_source_file            JSSC-2011-184-296.cif
_cod_data_source_block           Dy9B5S21
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_geom_angle_publ_flag' value 'N' was changed to 'n' in
accordance with the built-in table derived from the CIF Core
dictionary named 'cif_core.dic' version 2.4.5 last updated on
2014-11-21 (48 times).

data item '_geom_bond_publ_flag' value 'N' was changed to 'n' in
accordance with the built-in table derived from the CIF Core
dictionary named 'cif_core.dic' version 2.4.5 last updated on
2014-11-21 (26 times).

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_cell_volume        450.79(4)
_cod_database_code               1563308